**MODELING AND OPTIMIZATION OF FLANK WEAR AND SURFACE **

**ROUGHNESS OF MONEL-400 DURING HOT TURNING USING **

**ARTIFICIAL INTELLIGENCE TECHNIQUES **

*M. Hanief**, M. S. Charoo *

*Mechanical Engineering Department, National Institute of Technology Srinagar, *
*J&K,India*

*Received 29.01.2020 *
*Accepted 13.04.2020 *

**Abstract **

This work aims to model and investigate the effect of cutting speed, feed rate, depth
of cut and the workpiece temperature on surface roughness and flank wear (responses) of
Monel-400 during turning operation. It also aims to optimize the machining parameters
of the above operation. A power-law model is developed for this purpose and is
corroborated by comparing the results with the artificial neural network (ANN) model.
Based on the coefficient of determination (R2_{), mean square error (MSE), and mean }
absolute percentage error (MAPE) the results of the power-law model are found to be in
close agreement with that of ANN. Also, the proposed power law and ANN models for
surface roughness and flank wear are in close agreement with the experiment results. For
the power-law model *R2*_{, }* _{MSE, and }_{MAPE were found to be 99.83%, 9.9×10}*-4

_{, and }3.32×10-2

_{, and that of ANN were found to be 99.91%, 5.4×10}-4

_{, and 5.96×10}-2

_{, }respectively for surface roughness and flank wear. An error of 0.0642% (minimum) and 8.7346% (maximum) for surface roughness and 0.0261% (minimum) and 4.6073% (maximum) for flank wear were recorded between the observed and experimental results, respectively. In order to optimize the objective functions obtained from power-law models of the surface roughness and flank wear, GA (genetic algorithm) was used to determine the optimal values of the operating parameters and objective functions thereof. The optimal value of 2.1973 µm and 0.256 mm were found for surface roughness and flank wear, respectively.

**Keywords: **model; artificial neural network; genetic algorithm; flank wear;
surface roughness; turning.

**Introduction **

Hard turning is a turning of material with a hardness range from 45 to 68 HRC (Fig. 1). Hard turning has many advantages in addition to the cost of operation, such as faster metal removal rate, reduced cycle time, good surface finish and environmentally friendly, over grinding operation [1]. In machining, the material is strain-hardened due to the presence of retained austenite. The new machining industries aim to produce components at low product cost with good quality in minimum time. To achieve a good cutting performance in turning, the selection of optimum cutting parameters is important. Machinability of hardened materials was evaluated by cutting force for better surface roughness and tool wear by several researchers.

*Fig. 1. Turning operation on the lathe. *

However, turning the hard material to get a minimum surface roughness with
minimum tool wear is difficult. Katuku et al. [2] conducted experimental work in dry
cutting conditions on austempered ductile iron (ASTM Grade 2). The cutting forces, chip
characteristics and tool wear were analyzed with PCBN cutting tools. The result revealed
that the optimum cutting speed for better tool life and flank tool wear is 150 to 500 m/min.
In another work, *Marcelo Vasconcelos de Carvalho et al. [3] investigated the *
machinability of ADI (ASTM grades 2 and 3). It has been reported that minimum surface
roughness and higher tool wear observed when turning ADI grade3 with a higher tool
nose radius. In another work, Tuğrul Özel and Yiğit Karpat [4] developed the prediction
model using regression and neural networks in hard turning for surface roughness and
tool wear by CBN inserts. Minimum surface roughness was obtained at high workpiece
hardness with high cutting speed. Higher tool wear was obtained with the higher cutting
speed at lower feed rates. Lower feed rate gives a good surface finish. Zahia Hessainia et
*al. conducted experimental work on hard turning. The surface roughness was predicted *
with the use of cutting parameters and tool vibrations. The mixed ceramic cutting tool
Al2O3/TiC was used. They found that the feed rate was a more dominating factor than the

tool vibration in affecting the surface roughness [5]. *Mustafa Gunay and Emre Yuce *
applied the Taguchi method for cutting conditions optimizing for surface roughness in
turning of white cast iron (high alloy). Mandal et al. [6] investigated the optimization of
cutting parameters for tool flank wear using newly developed cutting tool Zirconia
Toughened Alumina (ZTA). Taguchi method and regression analysis were used to
optimize the cutting parameters. It has been observed that the tool wear was highly
affected by the depth of cut.

Nickel-based alloys have found wide applications ranging from automobile to the
aircraft sector owing to its properties such as excellent tensile strength, corrosion
resistance, ability to withstand elevated temperatures [7]. Monel-400, a solid solution of
Ni and Cu, is one of the nickel-based alloys in this category. Machining of such materials
by conventional methods encounters several problems which include rapid tool wear,
excessive cutting forces, more pronounced surface roughness [8]. The nickel-based alloys
have been machined by different machining operations-hard turning,
electro-discharge-machining etc. These electro-discharge-machining operations have limitations due to high cutting tool cost
and low (metal removal rate) MRR. Hot machining offers a good opportunity to machine
these alloys. Several investigations have been conducted by the researchers to study hot
machining. Parida and Maity [9] investigated the machinability of several nickel-based
alloys at elevated temperatures. The machinability in the hot condition was improved,
comparing the machinability at room temperature. The tool life was investigated by Ozler
*et al. [10] during the hot machining of high manganese steel using flame heating. It was *
found that the cutting speed has more effect on tool life than the feed rate and depth of
cut. *Ginta et al. [11] found that the machinability performance of titanium alloys at *
elevated temperatures is better as compared to that at room temperature. Similar results
have been reported by other researchers regarding the induction heat machining,
laser-assisted machining and plasma-laser-assisted machining [12]. Optimization of machining
parameters is necessary as it directly influences the cost, time and reliability of machining
operations. *Ranganathan and Senthilvelan [13] used a multi-objective optimization *
method in hot machining of AISI 316 using the grey Taguchi method. They took surface
roughness, material removal rate and tool life as system responses. Optimization of
machining parameters using flame heating has been studied by researchers in turning of
Monel-400 [14], Inconel 625 [13] and Ni-hard material [16] for improving machinability.
They used grey Taguchi, desirability, data envelopment analysis for optimization of
machining parameters. Zhang et al. [17] implemented a combined method of RSM and a
non-sorting genetic algorithm to optimize the wire-electro-discharge machining
parameters. Aouici et al. [18] applied surface response methodology to optimize the effect
of the cutting parameters on surface roughness, cutting force, specific cutting force, and
power consumption in hard turning of AISI D3 steel. Feed rate is the most influential
parameter affecting the cutting force and surface roughness compared to other
parameters. Gupta et al. [19] studied the mathematical modeling of surface roughness,
tool wear and power consumption in turning operation using surface response
methodology combined with artificial neural network and support vector regression.
*Aouici et al. [20] applied RSM to investigate cutting force and surface roughness by *
taking different hardness of AISI H11 steel. Koyee et al. [21] optimized the machining
parameters on flank wear, chip volume ratio, cutting force and cutting power using
response surface methodology combined with cuckoo search algorithm in turning duplex
steel. Parida [22] discussed the chip geometry in the hot machining of Inconel 718. He

concluded that chip geometry such as the degree of segmentation, serration frequency,
and equivalent chip thickness decreased with the increase of heating temperature.
*Venkatesh and Chandrakar [23] analyzed the heat-assisted turning of a nickel-base alloy. *
They concluded that heating on the surface of the workpiece reduces cutting force, surface
roughness and tool wear compared to room temperature machining. Nickel-based alloys
have been studied through experimental investigations and modeling by several
researchers but only one article could be found in the published literature on modeling of
hot machining of Monel-400 using response surface methodology. In order to have a
much better and more accurate model, power law and ANN have been used for modeling
the hot machining of Monel 400. The optimization of the machining operation has been
carried out through GA, where the power-law model has been used as an objective
function. Palani et al. [24] developed a mathematical model for Ra, tool wear ratio and
MRR in-terms of machining parameters and the model developed was used as desirability
function for carrying out the optimization of the machining parameters. *Durairaj and *
*Gowri [25] investigated the Ra and tool wear during the machining of Inconel-600 using *
a genetic algorithm for parametric optimization to improve tool life and surface finish. A
multi-pass turning parameter optimization was performed by *Rao and Kalyankar [26] *
using a teaching-learning based optimization algorithm. The results were compared with
GA and Particle swarm optimization techniques. *Asiltürk et al. [27] performed the *
optimization of parameters using Taguchi's method that influence Ra in Co28Cr6Mo
material. It was concluded that tooltip radius is the dominant factor that affects surface
quality. Selvakumar and Ravikumar [28] conducted optimization for minimum tool wear
and surface roughness during machining of Titanium alloy.

**Procedure and Modelling **

*Power-law model*

The relationship between the output, i.e. surface roughness and flank wear, and the machining parameters can be expressed as

𝑅𝑖= 𝐶𝑖. 𝑉𝑣𝑖. 𝐹𝑓𝑖. 𝐷𝑑𝑖. 𝑇𝑡𝑖 *1 *

𝑖 = 1, 2 where subscript 1 and 2 corresponds to surface roughness and flank wear. i.e. 𝑅1𝑎𝑛𝑑 𝑅2 are surface roughness and flank wear, 𝑉, is cutting speed, 𝐹 is feed rate, 𝐷 is the depth of cut, and 𝑇 is temperature. Unknown constants are 𝐶𝑖 , 𝑣𝑖, 𝑓𝑖 , 𝑑𝑖, 𝑎𝑛𝑑 𝑡𝑖 – determined from the experimental data. In order to find these constants, Eq. (1) is linearized by logarithmic transformation. We get

𝑙𝑛𝑅𝑖= 𝑙𝑛𝐶𝑖+ 𝑣𝑖𝑙𝑛𝑉 + 𝑓𝑖𝑙𝑛𝐹 + 𝑑𝑖𝑙𝑛𝐷 + 𝑡𝑖𝑙𝑛𝑇 *2 *
Eq. (2) can be rewritten as a linear mathematical model as

𝑅̅ = 𝐶𝑖̅ + 𝑣𝑖. 𝑉̅ + 𝑓𝑖. 𝐹̅ + 𝑑𝑖. 𝐷̅ + 𝑡𝑖. 𝑇̅ *3 *
where 𝐶̅ = 𝑙𝑛𝐶, 𝑉̅ = 𝑙𝑛𝑉, 𝐹̅ = 𝑙𝑛𝐹, 𝐷̅ = 𝑙𝑛𝐷 𝑎𝑛𝑑 𝑇̅ = 𝑙𝑛𝑇

using least square

we find the coefficients using Eq. (5) and the experimental data of Parida et al.
[30]. Where
𝛽𝑖=
[
𝐶𝑖
𝑣𝑖
𝑓𝑖
𝑑𝑖
𝑡𝑖]
*6 *
𝑋𝑖=
[
𝑎𝑟𝑟𝑎𝑦 𝑜𝑓 𝑖𝑛𝑝𝑢𝑡 𝑑𝑎𝑡𝑎
]
*7 *
*ANN model *

The capacity of ANN to solve nonlinear problems has attracted the attention of the researchers to solve the problems of machining. So, it has been used in this work too. ANN has many layers that depend on the complexity and type of problem. In general, it has an input layer, hidden layer and output layer. The input data are processed in the hidden layer. Next, the hidden layer computes the output and this is further processed in the output layer to produce the final results. The hidden layer and the output layer compute results based on the transfer functions. In this work, tansig and purelin functions were used as transfer functions in the hidden layer and output layer, respectively, and are given in Eqs. (8a) and (8b). The schematic representation of the ANN model is shown in Fig. 2.

𝐹(𝑥) =𝑒𝑥−𝑒−𝑥

𝑒𝑥_{+𝑒}−𝑥 *8a *

𝐹(𝑥) = 𝑥 *8b *

The ANN is initiated by training, where the input, along with the output, is introduced to the network, and the weights are set randomly. To achieve a satisfactory level of performance, weights are altered by the backpropagation algorithm to minimize the mean square error (MSE). In the backpropagation algorithm technique, the weights are adjusted by propagating weight changes back to the input neuron from the output neuron [29]. The training process is stopped when a satisfactory level of performance is attained. The network generated thereof uses these weights to make the decisions. The MATLAB toolbox was used for ANN modeling in this paper. The parameters used for the network are tabulated in Table 1.

*Table 1. Training parameters for the network. *
Number of neurons on the layer Input:1 hidden:2 output:1
Initial weights and biases Randomly between -1 and 1

Activation function Tansig

Learning rate 0.05

Momentum constant 0.95

Epochs 1000

Several independent runs with different initial random weights were performed to achieve the best possible solution. The MSE during the learning process of the network was evaluated by

𝑀𝑆𝐸 =∑𝑖=1𝑁 (𝑇𝑖−𝑂𝑖)2

𝑁 *9 *

where 𝑇 and 𝑂 are target and output values, respectively. The weights are again adjusted between the hidden and output layer and are calculated by Eq.(10)

∆𝑤𝑗𝑖(𝑛) − 𝛼∆𝑤𝑗𝑖(𝑛 − 1) + 𝜂𝛿𝑗(𝑛)𝑦𝑖(𝑛) *10 *
where ∆𝑤𝑗𝑖(𝑛) is the change in weights, 𝛼 is the momentum coefficient 𝛿𝑗(𝑛) is the
error, 𝜂 is the learning rate and 𝑦𝑖(𝑛) is the output. The results were tested with the
experimental data that were not presented during the training process after successful
training. The results were again compared with using R2 _{and MSE. R}2 _{is defined as the }
proportion of the variance in the dependent variable that is predicted from the independent
variable and is given by

𝑅2_{= 1 − (}∑𝑁𝑖=1(𝑇𝑖−𝑂𝑖)2

∑𝑁𝑖=1(𝑂𝑖)2

) *11 *

**Experimental setup and case study **

The experiments conducted by *Parida et al. [30] on Monel-400 to measure the *
surface roughness and flank wear were used for the present work. The tests were
performed on an HMT center lathe with 1200 rpm maximum speed and 6 kW spindle
power. A round bar of Monel-400 workpiece of diameter 40 mm and 300 mm length was
used in the experiments. A TiN coated inserts were utilized for machining operation
which was fitted to PSBNR 2525 M12 tool holder. To avoid error in the measurements,

each experimental run was carried out three times and a new cutting edge of the tool was used for each run. The flank wear of the cutting tool and roughness of machined surface were measured using an optical microscope and Taylor Hobson Surtronic S-100 Series surface roughness tester, with cut off value 0.8 mm.

**Results and discussion **

Power law and ANN model have been used for modeling surface roughness and flank wear during hot turning of Monel-400. The model parameters of the power-law equation were determined from experimental data. Also, the same data set was used for training and validation of the ANN model to carry out the comparison between the results of the two models (power law and ANN model). The Eq. (12) and (13) represent the model of the surface roughness and flank wear respectively.

𝑅𝑎= 5.6840 𝑉−0.1792_{ 𝐹}0.0568_{ 𝐷}0.0139_{ 𝑇}0.0029 * _{12 }*
𝐹𝑤 = 0.1633 𝑉0.1428

_{𝐹}0.0729

_{ 𝐷}0.0503

_{ 𝑇}−0.0007

*where 𝑅𝑎 and 𝐹𝑤 are surface roughness and flank wear, respectively.*

_{13 }From Eq. (12)
(𝜕𝑅𝑎
𝜕𝑉)_{𝐹,𝐷,𝑇}< 0,* *(
𝜕𝑅𝑎
𝜕𝐹)_{𝑉,𝐷,𝑇}> 0,* *(
𝜕𝑅𝑎
𝜕𝐷)_{𝑉,𝐹,𝑇}> 0,* and *(
𝜕𝑅𝑎
𝜕𝑇)_{𝑉,𝐹,𝐷}> 0* *

This implies that the surface roughness increases with feed rate, depth of cut and temperature but decreases with the increase in cutting speed.

Similarly, from Eq. (13)
(𝜕𝐹𝑤
𝜕𝑉)_{𝐹,𝐷,𝑇}> 0,* *(
𝜕𝐹𝑤
𝜕𝐹)_{𝑉,𝐷,𝑇}> 0,* *(
𝜕𝐹𝑤
𝜕𝐷)_{𝑉,𝐹,𝑇}> 0,* and *(
𝜕𝐹𝑤
𝜕𝑇)_{𝑉,𝐹,𝐷}< 0* *

Which implies that theflank wear increases with the increase in cutting speed, feed rate and depth of cut but decreases with an increase in temperature.

The temperature and cutting speed were found to be the most influential parameters that affect flank wear and surface roughness respectively.

The ANN was trained for 20 values of input and validated for 5 out of 30 experimental input data for both surface roughness and flank wear. The correlation of parameters of surface roughness and flank wear of the ANN model is given in Fig. 3.

*Fig. 3. Correlation of parameters for surface roughness and flank wear. *
Further, the comparison of surface roughness and flank wear with the experimental
results obtained from the power law and ANN are shown in Fig. 4 and Fig. 5 and Table
2. It can be seen from Fig. 4 and Fig. 5 that the maximum error for surface roughness is
about 8.5% and 4% for power law and ANN model, respectively. Similarly, the maximum
error for flank wear is about 20% and 17% power law and ANN model, respectively.

*Fig. 4. Comparison of proposed power law and ANN model with experimental results *
*for surface roughness. *

*Fig. 5. Comparison of proposed power law and ANN model with experimental results *
*for Flank wear. *

*Table 2. Statistical parameters of a proposed power law, ANN, and regression [30] *
*model. *

Surface roughness Flank wear

Power
law
ANN [30] Power
law
ANN [30]
R2 _{99.83% } _{99.91% } _{86.17% } _{98.72 } _{98.74 } _{94.72% }
MSE 0.0099 0.0054 0.0105 0.00081 0.00082 0.0025
MAPE 0.0332 0.0596 0.0377 0.094 0.0596 0.1151

**Optimization of machining parameters **

Multi-objective optimization, using the Genetic Algorithm (GA) is an efficient method for solving nonlinear and constrained problems. GA originated from the principle of natural genetics and been widely used for engineering problems, Zain et al. [31]. GA creates the Pareto Front with multiple outputs for optimal selection of parameters. The output of GA depends on the size of the population, selection type, GA operators i.e. mutation, and crossing over. In the present work, tournament selection was used to select individuals from the given population at random. Crossover involves a combination of two individuals to form parents or offspring for the next generation. While mutation causes random changes in the individual to widen search space for attaining genetic diversity. Adaptive feasible type function is used to select the search direction based on the last successful generation. Aim of multi-objective optimization in this work is to establish various optimum conditions for the chosen surface roughness and flank wear. The Eqs. (13) and (14) developed in the previous section by the power-law model are taken as the objective functions for optimization. Since, GA is based on maximum survival of best individuals, the objective functions for minimization of surface roughness, 𝑅𝑎 and 𝐹𝑤 has been taken directly. The objective functions Eq. (12) and (13) are subjected to the following boundary conditions:

40 ≤ 𝐶𝑢𝑡𝑡𝑖𝑛𝑔 𝑠𝑝𝑒𝑒𝑑 (𝑉) ≤ 100 0.1 ≤ 𝐹𝑒𝑒𝑑 𝑟𝑎𝑡𝑒 (𝐹) ≤ 0.15 0.5 ≤ 𝐷𝑒𝑝𝑡ℎ 𝑜𝑓 𝑐𝑢𝑡 (𝐷) ≤ 1 30 ≤ 𝑇𝑒𝑚𝑝𝑒𝑟𝑎𝑡𝑢𝑟𝑒 (𝑇) ≤ 600

The MATLAB toolbox was used for optimizing the objective functions. The Pareto front is shown in Fig. 6 and presented in Table 3. It consists of a set of possible solutions. Based on the priority given for each response variable, the particular combination is selected. In present work, equal priority is given to 𝑅𝑎 and 𝐹𝑤. The corresponding operating parameters are chosen as the optimum parameters. An optimum value of 𝑅𝑎 and 𝐹𝑤 were found to be 2.1973 and 0.2565, respectively. The corresponding parameters 𝑉 = 99.2758 mm/min, 𝐹 = 0.1014 mm/rev, 𝐷 = 0.5003𝑚𝑚, and 𝑇 = 92.9177 ℃.

*Table 3. Pareto front of GA. *

Input parameters Responses

Cutting speed (V) Feed rate (F) Depth of cut (D) Temperature (T) Surface roughness (Ra) Flank wear (Fw) 99.2758 40.2071 40.2071 51.7393 64.1634 85.0816 99.2758 87.8363 50.0571 73.6425 60.3162 91.5014 82.0776 71.0472 41.5800 61.2484 57.5948 68.8369 0.1014 0.1001 0.1001 0.1005 0.1022 0.1028 0.1014 0.1010 0.1013 0.1001 0.1008 0.1011 0.1015 0.1024 0.1001 0.1034 0.1071 0.1013 0.5003 0.5004 0.5004 0.5006 0.5038 0.5019 0.5003 0.5009 0.5010 0.5003 0.5010 0.5006 0.5005 0.5022 0.5011 0.5015 0.5039 0.5019 92.9177 130.5807 130.5807 112.2836 110.8685 104.0428 92.9177 98.1233 116.5851 112.6392 117.0805 94.5690 97.5883 127.7981 128.7734 112.6683 107.4933 105.5925 2.1973 2.5842 2.5842 2.4696 2.3786 2.2616 2.1973 2.2460 2.4856 2.3177 2.4033 2.2294 2.2739 2.3366 2.5688 2.4000 2.4313 2.3471 0.2565 0.2252 0.2252 0.2336 0.2412 0.2512 0.2565 0.2520 0.2326 0.2456 0.2388 0.2535 0.2497 0.2447 0.2263 0.2398 0.2384 0.2435

**Conclusion **

The models for surface roughness and flank wear, during the hot turning of Monel-400, are obtained using power law and ANN in this paper. The influences of machining parameters on surface roughness and flank wear have been analyzed based on proposed models. The optimal values of the machining parameters were determined by multi-objective optimization using a genetic algorithm. The power-law model developed was used as an objective function. The following conclusions were drawn from this work:

The 𝑅2_{, 𝑀𝑆𝐸 𝑎𝑛𝑑 𝑀𝐴𝑃𝐸}_{ of the power-law model were found to be }_{99.83%,}
9.9 × 10−4_{ and }_{3.32 × 10}−2_{, and that of ANN model were found to be }_{99.91%,}
5.4 × 10−4_{𝑎𝑛𝑑 5.96 × 10}−2_{, respectively. It was concluded from the above statistical }
parameters that the proposed models are competent to predict the surface roughness and
flank wear.

The surface roughness decreased with the increase of cutting speed and feed rate, whereas an increase in temperature and depth of cut caused an increase of the surface roughness.

An increase in cutting speed, feed rate and depth of cut, lead to an increase of flank wear. However, an increase in temperature up to a specific limit there decreased the tool wear and after that, the flank wear increased with the increase of temperature.

The temperature was the most influential factor which affects flank wear, whereas cutting speed was the most affecting factor influencing the surface roughness.

Using a genetic algorithm the optimal values of the machining parameters-cutting
speed, feed rate, depth of cut and temperature were found to be 99.2758 mm/min, 0.1014
mm/rev, 0.5003 mm and 92.9177 o_{C, respectively. The corresponding values of surface }
roughness (𝑅𝑎) and flank wear (𝐹𝑤) were found to be 2.1973 𝜇𝑚 and 0.2565 𝑚𝑚,
respectively.

**References **

[1] A. Srithar, K. Palanikumar, B. Durgaprasad: Procedia Engineering, 97 (2014) 72 – 77.

[2] K. Katuku, A. Koursaris and I. Sigalas: J Mater Process Technol, 209 (2009) 2412–2420.

[3] S. Yamamoto, H. Nakajima, H. Miyaji: Trans Iron Steel Inst Jpn, 81 (7), 2005, 721–726.

[4] T. Özel, Y. Karpat: International Journal of Machine Tools Manufacture, 45

(2005) 467–479.

[5] Z. Hessainia, A. Belbah, M.A. Yallese, T. Mabrouki, J.F. Rigal: Measurement, 46 (2013) 1671–1681.

[6] N. Mandal, B. Doloi, B. Mondal, R. Das: Measurement, 44 (2011) 2149–2155.

[7] E.O. Ezugwu: J Brazilian Soc Mech Sci Eng, 26 (2004) 1–11.

[8] E.O. Ezugwu, Z.M. Wang, A.R. Machado: J Mater Process Technol, 86 (1999) 1– 16.

[9] A.K. Parida, K.P. Maity: Adv Eng Forum, 16 (2016) 24-32.

[10] L. Özler, A. Inan, C. Özel: Int J Mach Tools Manuf, 41 (2001) 163–172.

[11] T.L. Ginta, A.K.M.N. Amin, M.A. Lajis, A.N.M. Karim, H.C.D.M. Radzi: Eur J

Sci Res, 27 (2009) 384–391.

[12] T.L. Ginta, A.K.M.N. Amin, A.N.M. Karim, A.U. Patwari, Modeling and optimization of tool life and surface roughness for end milling titanium alloy Ti – 6Al – 4V using uncoated WC-Co inserts, CUTSE Int. Conf. (2008) 24–27.

[13] S. Ranganathan, T. Senthilvelan: Int J Adv Manuf Technol, 56 (2011) 455–462.

[14] A.K. Parida, K.P. Maity: Int J Eng Res Africa, 24 (2016) 64–70.

[15] A.K. Parida, K.P. Maity: Int J Eng Res Africa, 24 (2016) 57–63.

[16] A.K. Parida, K.P. Maity: Adv Eng Forum, 16 (2016) 16–23.

[17] G. Zhang, Z. Zhang, W. Ming, J. Guo, Y. Huang, X. Shao: Int J Adv Manuf Technol, 70 (2014) 2097–2109.

[18] H. Aouici, H. Bouchelaghem, M.A. Yallese, M. Elbah, B. Fnides: Int J Adv Manuf Technol, 73 (2014) 1775–1788.

[19] A.K. Gupta: Int J Prod Res, 48 (2010) 763–778.

[20] H. Aouici, M.A. Yallese, K. Chaoui, T. Mabrouki, J. F. Rigal: Meas J Int Meas Confed, 45 (2012) 344–353.

[21] R.D. Koyee, U. Heisel, R. Eisseler, S. Schmauder: J Manuf Process, 16 (2014) 451–467.

[22] A.K. Parida: Iran J Sci Technol Trans Mech Eng, 43 (2018) 155–164.

[23] G. Venkatesh, D. Chandrakar: Silicon, 9 (2017) 867–877.

[24] S. Palani, U. Natarajan, M. Chellamalai: Mach Vis Appl, 24 (2013) 19–32.

[25] M. Durairaj, S. Gowri: Procedia Eng, 64 (2013) 878–887.

[26] R. Venkata Rao, V.D. Kalyankar: Scientia Iranica, 20 (2013) 967–974.

[27] I. Asiltürk, S. Neseli, M.A. Ince: Measurement, 78 (2016) 120–128. [28] S. Selvakumar, R. Ravikumar: Indian J Eng Mater Sci, 21 (2014) 397–408.

[29] M. Hanief, M. F. Wani: Applied Surface Science, 357 (2015) 1573-1577.

[30] A. K. Parida, K. Maity: Measurement, 137 (2019) 375–381.

[31] A.M. Zain, H. Haron, S. Sharif: Expert Syst Appl, 37 (2010) 4650–4659.